Effects of Waste Plastic on Cement Stabilized Soil
Prof. Rashmi Pantawane1, Aayushi Agrawal2, Girish Hatwar3, Vikesh Khobragade4, Vivek Chopade5, Pragat Sahare6 1
Assistant Professor, Department of Civil Engineering, J D College of Engineering & Management, Nagpur, Maharashtra. 2, 3, 4, 5, 6
UG Student, Department of Civil Engineering, J D College of Engineering & Management, Nagpur, Maharashtra.
Abstract: Soil adjustment is the procedure that improves soil physical properties, such as shear quality, bearing limit that should be possible through the use of controlled compaction or expansion of suitable admixtures such as cement, lime, sand, fly ash or geo-textiles, geo-synthetics, etc.
Expansive soils such as black cotton soil are always causing problems with swelling, shrinking and unequal foundation settlement. Black Cotton soils with high swelling and contracting potential are one of India's major soil deposits as a result of changes in moisture content.
The foundation is essential for any structure and it must be sufficiently able to help the whole structure. To establish the foundation, the soil around it plays a very important role in making plastic waste one of the world's biggest problems. . Utilization of plastic bottles and other plastic is exponentially expanding step by step because of these we are facing different ecological issues.
The new method of soil adjustment can be adequately used to address the difficulties of society, to reduce the amounts of waste, creating valuable material from non-helpful waste materials. A review paper is introduced here to focus on soil stabilization by utilizing waste plastic items. Tests such as liquid limit, plastic limit, standard proctor compaction test, California bear ratio (CBR) test and direct shear test were performed check improvement in the properties of black cotton soil. Different contents of plastic waste % by weight varying by 0.5% 1.0% and 1.5% The black cotton soil was added and the optimal percentage of plastic strips was determined by the California bearing test ratio. 2%, 4%, 6%, 8% and 10% cement is used as a stabilizer by weight of soil.
Keywords: Black cotton soil, Plastic waste, Cement, Soil Stabilization, California Bearing Ratio, Direct Shear test.
Soil is the most essential part of our daily lives. Human and animals uses soil for various purposes such as irrigation, which is an utmost importance for human survival. A large part of this existing soil is clayey type of soil which creates disturbance in the properties of soil.
The process of enhancing the various properties of soil in order to make it, more compatible is called as Stabilization. For the purpose of stabilization of clayey soil, a study on mixing of cement into the soil has been carried out and the considerable amount of rise in its shear strength was observed. To attain the desired amount of strength, a specific material called plastic which has better elastic properties is mixed in this soil. In this project work we have focused on the addition of plastic fiber mixed with cement to enhance the properties of the soil.
The use of plastic fiber results in increasing the durability of the soil while also maintaining its elastic properties. The plastic material which we are using is banned plastic in India which also helps to reduce the harsh effects on environment by this project. Utilization of cement in this project helps strengthen the binding properties of the soil. If this method is adopted at site it will surely make the entire construction work economical.
The inclusion of plastic fiber will intersect the failure plane which will ultimately provide resistance to shear when the soil is subjected to any loading. The reinforced soil obtained by applying the concept derived through this project can be used as a subgrade material for the pavement as well as in case of foundation trenches.
The aim of the project is to stabilize the soil for improving the various properties such as shear strength, bearing capacity by using different mixes of plastic strips and cement. Soil type was determined by examine of various soil parameters like OMD, MDD, Atterberg’s limit and Wet sieve analysis.
III. PROCESS PLAN
Expansive soils in India popularly known as black cotton soils are among the problem soils from the point of view of civil engineering. The basic mineralogical composition is very important of the different factors affecting the soil's swelling behaviors. Most of the expansive soil is rich in mineral, montmorillonite, and some in illite. The soil's most important characteristics are that it shrinks when dry and is hard and has very high bearing capacity. Large cracks form in the soil, but expand when the soil is moist and loses capacity
Cement is a binding material used for construction. Various grades of cement are available in the market as we studied such as OPC 43 & 53 grade etc. Cement has hydrating properties which results in even setting and hardening under water. Here, we are using OPC 53 grade of cement for this project.
Properties of OPC 53 Grade Cement
Sr.No. Properties Typical range Result IS Code I. Consistency (%) 26-33% 27.5 IS 4031- 4 II. Setting time
Initial (minutes) Final (minutes)
30 – 600 min 125 250
IS 4031- 5
III. Soundness (mm)
(by Le-Chat Expansion) -- 1.0
IS 4031- 3 IV. Comp. Strength (kg/sq.cm)
7 days 28 days
C. Plastic Strips
Properties Of Plastic Strips
Diameter / Width 2 mm
Length 15 mm
Tensile Strength 32 N/mm2 Flexural Strength 41 N/mm2
Elongation 40-100 N/mm2
V. TESTS TO BE PERFORMED ON NORMAL SOIL
A. Mix Proportion
Weighing batching is adopted and mixing combinations (total 7 nos) in the proposed work were planned
Soil 98% 96% 94% 92% 90%
Cement 2% 4% 6% 8% 10%
Mix Proportions For Optimum Cement-Soil And Plastic Fibre Material Values in percentage contribution of sample
Soil 90% 90% 90%
Cement 10% 10% 10%
Plastic 0.5% 1% 1.5%
B. Wet sieve analysis
Wet sieve Analysis is a procedure that is generally used to assess the distribution or gradation of particle size of a granular material. It is also used to prepare a granular material for analysis of particle size by removing fines that may impede the process of
Wet Sieve Analysis
Sieve Empty sieve With sieve after oven dried Final Reading 10 mm 67 gm 0 gm 0 gm 4.75 mm 360 gm 420 gm 60 gm 2.36 mm 300 gm 340 gm 90 gm 1.18 mm 310 gm 440 gm 130 gm 600 μ 320 gm 330 gm 10 gm 2.13mm 300 gm 320 gm 20 gm 75μ 270 gm 270 gm 10gm Pan 280 gm 290 gm -
Result: Gravel= 3% Sand = 15% Silt & Clay= 82%
0 20 40 60 80 100
0.00 0.01 0.10 1.00 10.00 100.00
0.002 0.075 4.75
D. Core Cutter Test
This method is used to determine the dry density of soil. It is need to determine the stability analysis of slopes, bearing capacity of soil and the design of underground structures. It is very quality control test, compaction is required.
Results: Field density of core cutter = 1.95 gm/cc
V. RESULTS AND DISCUSSIONS
A. Test And Results On Soil
Properties of Black Cotton Soil Sr.
No. Properties Typical range Observed IS code
I. Silt & clay content (%) 40-60 82% IS (2720-4)
II. Liquid limit (%) 50-60 63.41 IS (2720-4)
III. Plastic limit (%) 25-40 27.12 IS (2720-6)
IV. Shrinkage limit 9-18 10.77 IS (2720-6)
V. Specific gravity 2.6- 2.8 2.63 IS (2720-4)
VI. Standard Proctor Test
Maximum Dry Density (g/cc) 1.4-1.8 1.749 IS (2720-7) Optimum Moisture Content (%) 15-30 16.4 IS (2720-7) VII. California Bearing Ratio (%) 2 – 6 % 2.341 IS (2720-16)
B. Test And Results On Cement Stabilized Soil
Various doses of cement are added into black cotton soil and all the tests were performed to analyses the strength of black cotton soil.
Tests On Black Cotton Soil Using Cement Virgin
Cement addition by weight
2% 4% 6% 8% 10%
Liquid limit 65.25 65.01 63.92 60.02 59.01 55.92
Plastic Limit 28.15 30.88 37.89 38.01 38.21 37.11
Maximum dry density 1.749
g/cc 17.22 17.41 17.86 18.22 18.60 Optimum moisture
content 16.4% 1.745 1.743 1.741 1.738 1.701
IP 37.1 34.13 26.03 22.01 20.8 18.81
OMC & MDD
0.2 5.2 10.2 15.2 20.2 25.2
0 5 10 15
O p ti m u m m o is tu re c o n te n t (% )
% DOSE OF CEMENT
PROCTOR 0.2 0.7 1.2 1.7 2.2
0 5 10 15
D R Y D EN SI TY ( G M /C C )
% DOSE OF CEMENT
C. CBR Results For Different Doses Of Self - Contained Cement
Sr. No Sample 0 days 7 days 14 days 28 days
I. Soil 2.341 - - -
II. Soil+ 2% c 2.383 2.431 3.652 4.028
III. Soil+ 4% c 2.461 3.784 4.881 5.573
IV. Soil+ 6% c 2.535 4.743 5.941 6.742
V. Soil+ 8% c 2.787 5.179 6.476 7.474
VI. Soil+ 10% c 3.142 5.817 7.162 8.264
CBR results for various doses of cement with soil and 0.5%,1.0%,1.5% plastic fibre
CBR result 10% with plastic fibre
Soil + 2% C Soil + 4% C Soil + 6% C Soil + 8% C Soil + 10% C
Doses of cement
Graph: CBR result for cement stabilized soil
Soil + 10% C+0.5% Plastic
Soil + 10% C+1.0% Plastic
Soil + 10% C+1.5% Plastic
Graph: CBR result for 10% C+Plastic fibre
Sr No. Optimum limit Nomenclature 0 Days (%)
7 Days (%)
14 Days (%)
28 Days (%)
I soil +10% cement
5.762 8.763 10.481 12.174
6.441 9.574 11.523 13.183
Results Of Normal Soil With Cement
Sr.no Nomenclature Liquid Limit Plastic Limit Plasticity Index
I. S0 65.12 28.15 36.97
II. S0+ 2%C 65.01 30.88 34.13
III. S0+4%C 63.92 37.89 26.03
IV. S0+6%C 60.02 38.01 22.01
V. S0+8%C 59.01 38.21 20.8
VI. S0+10%C 55.92 37.11 18.81
D. Direct Shear Test
Direct shear is defined as a test which is performed to get the shear strength value of soil .Mostly test has been performed by drained and un-drained soil.
The purpose of the soil's direct shear test is to obtain its ultimate shear resistance, inner friction angle, cohesion, and deformation characteristics of shear stress.
E. Result of Direct Shear Test
Direct shear result for soil + 10% Cement & 0.5%, 1.0 % & 1.5 % Plastic waste.
Sr No. Specimen Load in Kg Shear stress(kg/cm2)
I. Normal soil 1 0.5
II. Soil + 10 % cement +0.5% Plastic waste 1 0.63
III. Soil + 10 % cement +1.5% Plastic waste 1 0.68
Vertical gauge = 0.01mm Horizontal gauge =0.01mm
Proving gauge =0.002-5mm Calibration factor =0.262 (constant) Dry density of soil =1.95 gm/cc Volume of mould =6*6*2.5=90cm3 Weight of soil =1.95*90=175.5 gm
VII. RESULTS AND DISCUSSIONS
We have studied all the various tests conducted on this project. Now, here we are going to do a comparative study on plastic waste and cement mixed with the soil. Firstly, we performing tests on normal soil and another tests with plastic fiber mixed soil. We compare both the values in tests and observe the change in their properties. We noticed and came to the results that the soil which is mixed with plastics is having better strength and having good elastic properties as compared to the normal soil without any admixture.
A. Shear strength is one of the most important parameter of the soil which ultimately reflects the quality of soil.
B. When the soil was reinforced with cement and plastic fibre a rise in its shear strength was observed at a considerable rate.
C. The main aim of this project was to make the clayey soil more stable in order to sustain the applied load from getting sheared.
D. Shear strength of soil increased when the percentage of additives was changed where the change was in terms of increasing the quantity of additives.
E. Till now the tests on reinforced soil with a decided proportion is conducted and there are some variations in proportions which are yet to be made.
F. The remaining variations are to be done very shortly.
 Consoli, N.C., Scapini, B., Festugato, L., 2013a. A practical methodology for the determination of failure envelopes of fiber-reinforced cemented sands. Geotext. Geomemb. 41, 50e54.
 Consoli, N.C., Moraes, R.R., Festugato, L., 2013b. Parameters controlling tensile and compressive strength of fiber-reinforced cemented soil. J. Mater. Civ. Eng. 25 (10), 1568e1573.
 Consoli, N.C., Moraes, R.R., Festugato, L., 2013c. Variables controlling strength of fibre-reinforced cemented soils. Ground Improv. 166 (4), 221e232.  Custodio, D.G., 2013. Mechanical behaviour of a stabilized soft soil with poly- propylene fibres. M.Sc. dissertation. University of Coimbra, Coimbra, Portugal
 Festugato, L., Fourie, A., Consoli, N.C., 2013. Cyclic shear response of fibre-reinforced cemented paste backfill. Geotech. Lett. 3, 5 e12.
 Hamidi, A., Hooresfand, M., 2013. Effect of fiber reinforcement on triaxial shear behavior of cement treated sand. Geotext. Geomemb. 36, 1e9. Hernandez-Martinez,
 Kitazume, M., Terashi, M., 2013. The Deep Mixing MethoddPrinciple, Design and Construction. Coastal Development Institute of Technology.  Estabragh, A.R., Namdar, P., Javadi, A.A., 2012. Behavior of cement-stabilized clay reinforced with nylon fiber. Geosynth. Int. 19 (1), 85e92.
 Correia, A.A.S., 2011. Applicability of Deep Mixing Technique to the Soft Soil of Baixo Mondego. Ph.D. dissertation. University of Coimbra, Coimbra, Portugal (in Portuguese).
 Consoli, N.C., Bellaver Corte, M., Festugato, L., 2011. Key parameter for tensile and compressive strength of fibre-reinforced soil-lime mixtures. Geosynth. Int. 19 (5), 409e414.
 Consoli, N.C., Zortea, F., Souza, M., Festugato, L., 2011a. Studies on the dosage of fiber-reinforced cemented soils. J. Mater. Civ. Eng. 23 (12), 1624e1632.  Consoli, N.C., Moraes, R.R., Festugato, L., 2011b. Split tensile strength of monofilament polypropylene fiber-reinforced cemented sandy soils. Geosynth. Int.
18 (2), 57e62.
 Venda Oliveira, P.J., Lemos, L.J.L., Coelho, P.A.L.P., 2010. Behavior of an atypical embankment on soft soil: field observations and numerical simulation. J. Geotech. Geoenviron. Eng. 136 (1), 35e47.
 Al-Tabbaa, A., Barker, P., Evans, C.W., 2009. Keynote lecture: design of deep mixing in infrastructure applications. In: International Symposium of Deep Mixing & Admixture Stabilization. Okinawa, Japan.
 F.G., Sparrevik, M., Kvalvåg, f., Eggen, A., Kvennås, A., Grini, R.S., 2009. Stabilization/solidification of two contaminate marine sediments. In: International Symposium of Deep Mixing &Admixture Stabilization. Okinawa, Japan.
 Terashi, M., Kitazume, M., 2009. Keynote lecture: current practice and future perspective of QA/QC for deep-mixed ground. In: International Symposium of Deep Mixing &Admixture Stabilization. Okinawa, Japan.
 Chauhan, M.S., Mittal, S., Mohanty, B., 2008. Performance evaluation of silty sand subgrade reinforced with fly ash and fibre. Geotext. Geomemb. 26 (5), 429e435.
 Khattak, M.J., Alrashidi, M., 2006. Durability and mechanistic characteristics of fiber reinforced soil-cement mixtures. Int. J. Pavement Eng. 7 (1), 53e62.  Janz, M., Johansson, S.-E., 2002. The Function of Different Binding Agents in Deep Stabilization. Swedish Deep Stabilization Research Centre, Report 9,
Linkoping, € Sweden.
 Eurosoilstab, 2001. Development of Design and Construction Methods to Stabilise Soft Organic Soils. Design Guide Soft Soil Stabilization, p. 94. CT97-0351, EC Project No. BE 96-3177, Industrial & Materials Technologies Programme (BriteEuRam III), European Commission.
 Kaniraj, S.R., Havanaji, V.J., 2001. Behavior of cement-stabilized fiber- reinforced fly ash-soil mixtures. J. Geotech. Geoenviron. Eng. 127 (7), 574e584.  Federal Highway Administration, Washington, DC. EN 197-1, 2000. Cement e Part 1: Composition, Specifications and Conformity Criteria for Common
Cements. European Committee for Standardization, June 2010